- Review Article
- Open Access
Trunnionosis in total hip arthroplasty: a review
Journal of Orthopaedics and Traumatology volume 17, pages 1–6 (2016)
Trunnionosis is defined as wear of the femoral head–neck interface and has recently been acknowledged as a growing cause of total hip arthroplasty failure. Some studies have reported that it accounts for up to 3 % of all revisions. The exact cause of trunnionosis is currently unknown; however, postulated etiologies include modular junction wear, corrosion damage, and metal ion release. Additionally, implant design and trunnion geometries may contribute to the progression of component failure. In order to aid in our understanding of this phenomenon, our aim was to present the current literature on (1) the effect of femoral head size on trunnionosis, (2) the effect of trunnion design on trunnionosis, (3) localized biological reactions associated with trunnionosis, and (4) gross trunnion failures. It is hoped that this will encourage further research and interest aimed at minimizing this complication.
Trunnionosis is defined as the wear of the femoral head–neck interface and has been acknowledged as a source of total hip arthroplasty (THA) failure . This phenomenon appears to have gained prevalence with newer THA implant designs, particularly when modularity was introduced. Modularity allows for a better intraoperative restoration of leg length and control of hip offset , but while this enables a more customized fit for the patient, it may have untoward effects. The modularity at times may play a role in increased wear and mechanical insufficiency at the trunnion, ultimately leading to revision . In fact, trunnionosis is estimated to account for up to 3 % of all THA revision procedures [4, 5].
The exact cause of trunnionosis, which is likely multi-factorial, currently remains poorly understood. It is postulated that contributing factors include wear between metal-on-metal modular junctions , corrosion and fretting damage , and the release of metal ions or particulate debris from affected components . Additionally, different implant designs and geometries have demonstrated a predisposition to trunnion failure .
Multiple studies have postulated on the causes of trunnionosis. Therefore, we will examine the current literature and collate the evidence on trunnionosis following THA. Specifically, we present the literature on (1) the effect of femoral head size on trunnionosis, (2) the effect of trunnion design on trunnionosis, (3) localized biological reactions associated with trunnionosis, and (4) gross trunnion failures.
We performed a literature search using PubMed, EBSCO Host, and SCOPUS. We searched studies from inception of the respective databases up to September 2015 using various combinations of the following search terms—‘trunnion’, ‘THA’, ‘total hip arthroplasty’, ‘taper’, ‘wear’, ‘trunnionosis’, ‘hip’, ‘corrosion’, ‘fretting’, ‘ARMD’, ‘junction’, ‘ALTR’, ‘debris’, and ‘component’.
We reviewed 102 abstracts to determine articles that were appropriate for this review. We identified 70 potentially relevant articles for further evaluation. We excluded 45 articles that were not in English or not relevant to the topic. We then assessed the references of articles and found an additional 11 reports. We included four articles discussing femoral head sizes, four articles discussing trunnion design, six articles discussing local biological reactions, and four articles discussing gross trunnion failure.
Large-diameter femoral heads
The introduction of large-diameter femoral heads was postulated to decrease component instability while also increasing the impingement-free range-of-motion. However, larger femoral heads have been considered to cause an increase in the effective horizontal lever arm, which imparts greater torsional forces at the head–neck junction  (Table 1).
In a finite elemental analysis model assessing five trunnion–head junctions, Lavernia et al.  determined that not only was the area of maximum stress located on the medial aspect of the femoral neck, but also that the maximum stress in this area increased with larger head diameters. Maximum principal stresses for 28-, 32-, and 40-mm cobalt-chromium (CoCr) heads were 20.3, 36.0, and 43.8 megapascals (MPa), respectively. Stress increases within the trunnion were also computed. The trunnions for the 28-, 32-, and 40-mm CoCr heads exhibited stresses of 10.1, 12.1, and 16.6 MPa, respectively, in the central area of the trunnion adjacent to the femoral head. The authors concluded that stress levels were directly correlated to femoral head diameter. This may imply that the increased forces at the trunnion exerted by larger diameter heads play a role in component failure. Bolland et al.  published high failure rates after examining a cohort of 199 hips (185 patients) with large-diameter (>38 mm) hybrid THAs. At a mean follow-up of 62 months, 17 hips (8.5 %) had undergone a revision, with 14 more awaiting surgery. Between all hips that were revised or awaiting revision, the mean femoral head diameter was 46 mm (range 40–54 mm). During revision surgery, retrieved components displayed corrosion of the stem surface as well as increased wear at the head–neck junction. Dyrkacz et al.  found a significant difference in corrosion scores in the bore taper of a 36-mm head (15 hips) compared to a 28-mm head (59 hips) (P = 0.022) in a retrieval analysis to determine the effect of head size on corrosion and fretting in modular THA prostheses. When comparing the relationship between the heads and necks for corrosion damage, the 36-mm group demonstrated a greater correlation compared to the 28-mm group (0.975 vs 0.502). The 36-mm group also exhibited a greater correlation for head and neck fretting damage (1.0 vs 0.366).
Conversely, some studies have described how large-diameter femoral heads may not have a significant effect on damage at the trunnion–taper junction. In a retrospective study examining 110 large-diameter (>36 mm) THAs, Matthies et al.  demonstrated that the volume of material loss was negligible (<1 mm3) in the trunnions of all 36 femoral stems that were received. In fact, the median volume loss (0.29 mm3) was significantly less than that of the female taper, the femoral head, and acetabular-bearing surfaces (P < 0.001 for all). However, for the trunnions in this study, it should be noted that a significant positive correlation was observed between corrosion score and volume of material loss (ρ = 0.72, 95 % CI = 0.44–0.87, P < 0.001). Triantafyllopoulos et al.  conducted a retrieval analysis of 154 THAs. Ultimately, they found no association between femoral head size and the degree of fretting and corrosion on tapers (P = 0.247; P = 0.837, respectively) or trunnions (P = 0.471; P = 0.868, respectively). While this type of damage may be a regular occurrence in THAs, neither fretting nor corrosion was associated with femoral head size.
In summary, the association between large-diameter femoral heads and increased trunnion wear is inconclusive. While large femoral head may potentially cause elevated trunnion stresses, future studies should investigate if other factors, such as alloy composition, have greater responsibility.
The geometries of different trunnion designs may contribute to trunnionosis, as they influence torsional forces at the trunnion–taper interface . Recently, trunnions have become shorter in length in an effort to increase the impingement-free range-of-motion (Table 2).
Unfortunately, a shorter trunnion requires that its base sits within the taper of the femoral head, which may increase the likelihood of edge loading. Tan et al.  previously described this effect on the base in a retrieval analysis of 44 implants. When evaluating different regions of the trunnion, the authors noted significantly greater corrosion scores within the base zone (P = 0.018). They concluded that the base zone is subject to higher mechanical loading and greater torque forces compared to other regions. Brock et al.  retrieved 104 female tapers and 11 stem trunnions from 98 patients who experienced adverse reaction to metal debris. The authors used a co-ordinate measuring machine to assess for linear and volumetric wear of either shorter 12-mm/14-mm threaded trunnions or longer, smoother 11-mm/13-mm trunnions. They were able to identify significantly higher rates of material loss with the shorter, threaded 12-mm/14-mm trunnions compared to the longer, smooth 11-mm/13-mm trunnions (0.402 vs 0.123 mm3/year; P = 0.035). Porter et al.  conducted a retrieval analysis of 85 modular femoral stems released between 1983 and 2012 to determine how trunnion flexural rigidity and length have changed over time. They found a negative correlation between flexural rigidity (−0.23; P = 0.04) and trunnion length (−0.53; P < 0.001) with release date of the stem. Additionally, multiple regression analysis showed that flexural rigidity (β = −0.17) and trunnion length (β = −0.051) were independently correlated with time. Investigation of components in this study demonstrated that as new femoral stems were introduced, trunnions became less rigid and shorter.
Trunnion diameters have also been trending towards slimmer measurements in an effort to avoid impingement, i.e., from the older 14-mm/16-mm diameter to the more widely used 12-mm/14-mm diameter. It is thought that a decreased trunnion diameter translates to a reduced surface area for contact length and fitting, and therefore, increases the possibility for these complications [9, 17]. Contrary to this, a retrospective retrieval study by Nassif et al.  examined a small group of failed implants and revealed that thicker tapers with longer contact lengths were associated with greater fretting scores. Trunnions with 11-mm/13-mm tapers demonstrated significantly higher fretting scores compared to the narrower type one tapers (P = 0.005). This study also included 12-mm/14-mm tapers, but showed no significant association with fretting or corrosion scores. This particular investigation is limited because it examined a small group of failed implants from a heterogeneous cohort with respect to taper–trunnion geometry, alloy composition, implant manufacturer, and reason for revision.
In summary, many studies show how large femoral head diameters and shorter trunnion lengths might affect component damage. More research is necessary, as results concerning the effects of trunnion design still have to be considered inconclusive at present.
Local biological reactions
Local soft-tissue reactions have been observed as a result of corrosion debris produced at the trunnion [19, 20]. The clinical and histological appearance seen in periprosthetic tissue reactions surrounding corroded trunnions is similar to that of adverse local tissue reactions (ALTRs) seen in defective metal-on-metal (MoM) [21, 22] and non-MoM [22, 23] bearings. Adverse biologic reactions related to metal components include necrosis, lymphocytosis, vasculitis, and production of exudates, pseudotumors, or sinuses [24–26]. Pseudotumors, which are non-malignant soft-tissue growths due to particulate debris irritation , have a histological appearance reflecting that of metal wear reactions and metal hypersensitivity. Many reports describing ALTRs note the use of implants containing cobalt, a metal that is known to have a more deleterious effect on macrophages compared to other metals found in implants . These distinct tissue reactions have also been termed adverse reaction to metal debris (ARMD)  or aseptic lymphocyte-dominated vasculitis-associated lesions (ALVAL) . It is possible that corrosion and ion release at the trunnion may be a provoking factor.
Several studies have described ALTRs related to trunnion wear (Table 3). In a case series examining ten THAs, Cooper et al.  described how the femoral head–neck junction in all patients contained a black, flaky material at the trunnion. Moreover, the surgeons encountered large amounts of white to brownish fluid, hypertrophic synovial tissue, and pseudotumors in several cases. One patient who demonstrated pseudotumor formation suffered from subsequent dislocations due to moderate hip abductor muscle necrosis that eventually required a second revision. In a study by Gill et al.  of 35 patients who received modular THAs, three patients presented with postoperative pain secondary to pseudotumor formation as a result of corrosion at the head–neck interface. Histological analysis demonstrated ALVALs of the periprosthetic tissue. Upon retrieval analysis, corrosion was seen at the trunnions in two implants. Lindgren et al.  described a patient with an uncemented hip prosthesis who required revision secondary to pain, swelling, and recurrent head dislocation. Intraoperatively, pseudotumor formation and local soft-tissue destruction were identified, which were suspected to result from the corrosion observed at the trunnion–taper junction. Hsu et al.  presented a case of pseudotumor formation secondary to corrosion at the head–neck junction in a ceramic-on-polyethylene THA. The mass also extended around the greater trochanteric bursa and enveloped the short external rotators, resulting in moderate damage to the muscle attachments. Frozen sections showed signs of chronic inflammation and synovial necrosis. Stahnke and Sharpe  described a patient who presented with a large (12-cm diameter) pseudotumor and abductor muscle damage. Intraoperatively, metal wear was identified at the trunnion and histological analysis showed the presence of ALVALs.
Gross trunnion failure
The mechanisms leading to gross trunnion failure are largely unknown; however, its manifestations have been reported in several studies (Table 4).
Banerjee et al.  reported a case series of five patients who presented with gross trunnion failure after primary THA, necessitating revision. In this report, gross trunnion failures were defined as trunnions that exhibited a fracture or gross loss of material volume upon revision. All patients received modular components from five different manufacturers with femoral head diameters ranging from 28- to 40-mm. The authors were unable to locate a common link among these patients. However, it was suspected that the trunnion failures were due to a combination of patient, surgical, and component factors such as comorbidities, trunnion composition, skirted necks, formation of heterotopic ossification, and component damage during insertion. Hohman et al.  described a case of a THA that failed 3 years postoperatively. Intraoperative findings included a damaged liner insert, an intact femoral head, diffuse metallic debris, and excessive wear of the trunnion. Additionally, Pansard et al.  reported a patient who had unexplained pain at 2 years following THA and was found to have asymmetric fit of the trunnion and head on radiographic imaging. During revision, abnormal mobility was found between the femoral head and the 12-mm/14-mm trunnion, with severe damage at the taper. Further examination of the trunnion showed macroscopic pitting and wear. Histological analysis of periprosthetic tissues showed inflammatory infiltration of lymphocytes, plasmocytes, and multinucleate giant cells containing fine black particles indicative of metallosis. Botti et al.  presented a patient who suffered from trunnion fracture 14 years after the index THA, with no preceeding trauma. Upon retrieval analysis, it was determined that the fracture surface exhibited characteristics of pitting and crevice corrosion. Black metallic debris was also observed on the proximal region of the femoral stem, which was suspected to be caused by repetitive contact of the fractured surfaces.
Trunnionosis is a well-known cause of failed total hip arthroplasties. While contributing elements may include corrosion, mechanical stress, and particular implant designs, the exact origin of trunnionosis remains poorly understood. There is growing evidence to suggest that orthopedists should be aware of soft-tissue reactions as well as signs of trunnion failure in patients who have received a THA. Moreover, continued analysis of periprosthetic tissues and retrieved implants is fundamental for understanding how patient factors influence the cellular response to corrosion debris.
Pastides PS, Dodd M, Sarraf KM, Willis-Owen CA (2013) Trunnionosis: a pain in the neck. World J Orthop 4(4):161
Banerjee S, Cherian JJ, Bono JV, Kurtz SM, Geesink R, Meneghini RM, Delanois RE, Mont MA (2015) Gross trunnion failure after primary total hip arthroplasty. J Arthroplasty 30(4):641
Lavernia CJ, Iacobelli DA, Villa JM, Jones K, Gonzalez JL, Jones WK (2015) Trunnion-head stresses in THA: are big heads trouble? J Arthroplasty 30(6):1085
Porter DA, Urban RM, Jacobs JJ, Gilbert JL, Rodriguez JA, Cooper HJ (2014) Modern trunnions are more flexible: a mechanical analysis of THA taper designs. Clin Orthop Relat Res 472(12):3963
Drummond J, Tran P, Fary C (2015) Metal-on-metal hip arthroplasty: a review of adverse reactions and patient management. J Funct Biomater 6(3):486
Pivec R, Meneghini RM, Hozack WJ, Westrich GH, Mont MA (2014) Modular taper junction corrosion and failure: how to approach a recalled total hip arthroplasty implant. J Arthroplasty 29(1):1
Gilbert JL, Buckley CA, Jacobs JJ (1993) In vivo corrosion of modular hip prosthesis components in mixed and similar metal combinations. The effect of crevice, stress, motion, and alloy coupling. J Biomed Mater Res 27(12):1533
Langton DJ, Jameson SS, Joyce TJ, Gandhi JN, Sidaginamale R, Mereddy P, Lord J, Nargol AV (2011) Accelerating failure rate of the ASR total hip replacement. J Bone Joint Surg Br 93(8):1011
Langton DJ, Sidaginamale R, Lord JK, Nargol AV, Joyce TJ (2012) Taper junction failure in large-diameter metal-on-metal bearings. Bone Joint Res 1(4):56
Bolland BJ, Culliford DJ, Langton DJ, Millington JP, Arden NK, Latham JM (2011) High failure rates with a large-diameter hybrid metal-on-metal total hip replacement: clinical, radiological and retrieval analysis. J Bone Joint Surg Br 93(5):608
Dyrkacz RM, Brandt JM, Ojo OA, Turgeon TR, Wyss UP (2013) The influence of head size on corrosion and fretting behaviour at the head–neck interface of artificial hip joints. J Arthroplasty 28(6):1036
Matthies AK, Racasan R, Bills P, Blunt L, Cro S, Panagiotidou A, Blunn G, Skinner J, Hart AJ (2013) Material loss at the taper junction of retrieved large head metal-on-metal total hip replacements. J Orthop Res 31(11):1677
Triantafyllopoulos GK, Elpers ME, Burket JC, Esposito CI, Padgett DE, Otto Wright TM (2015) Aufranc award: large heads do not increase damage at the head–neck taper of metal-on-polyethylene total hip arthroplasties. Clin Orthop Relat Res 474(2):330–338
Cales B, Stefani Y (1998) Risks and advantages in standardization of bores and cones for heads in modular hip prostheses. J Biomed Mater Res 43(1):62
Tan SC, Teeter MG, Del Balso C, Howard JL, Lanting BA (2015) Effect of taper design on trunnionosis in metal on polyethylene total hip arthroplasty. J Arthroplasty 30(7):1269
Brock TM, Sidaginamale R, Rushton S, Nargol AV, Bowsher JG, Savisaar C, Joyce TJ, Deehan DJ, Lord JK, Langton DJ (2015) Shorter, rough trunnion surfaces are associated with higher taper wear rates than longer, smooth trunnion surfaces in a contemporary large head metal-on-metal total hip arthroplasty system. J Orthop Res 33(12):1868–1874
Hussenbocus S, Kosuge D, Solomon LB, Howie DW, Oskouei RH (2015) Head–neck taper corrosion in hip arthroplasty. Biomed Res Int 2015:758123
Nassif NA, Nawabi DH, Stoner K, Elpers M, Wright T, Padgett DE (2014) Taper design affects failure of large-head metal-on-metal total hip replacements. Clin Orthop Relat Res 472(2):564
Urban RM, Jacobs JJ, Gilbert JL, Galante JO (1994) Migration of corrosion products from modular hip prostheses. Particle microanalysis and histopathological findings. J Bone Joint Surg Am 76(9):1345
Jacobs JJ, Urban RM, Gilbert JL, Skipor AK, Black J, Jasty M, Galante JO (1995) Local and distant products from modularity. Clin Orthop Relat Res 319:94
Campbell P, Ebramzadeh E, Nelson S, Takamura K, De Smet K, Amstutz HC (2010) Histological features of pseudotumor-like tissues from metal-on-metal hips. Clin Orthop Relat Res 468(9):2321
Mahendra G, Pandit H, Kliskey K, Murray D, Gill HS, Athanasou N (2009) Necrotic and inflammatory changes in metal-on-metal resurfacing hip arthroplasties. Acta Orthop 80(6):653
Gill IP, Webb J, Sloan K, Beaver RJ (2012) Corrosion at the neck-stem junction as a cause of metal ion release and pseudotumor formation. J Bone Joint Surg Br 94(7):895
Davies AP, Willert HG, Campbell PA, Learmonth ID, Case CP (2005) An unusual lymphocytic perivascular infiltration in tissues around contemporary metal-on-metal joint replacements. J Bone Joint Surg Am 87(1):18
Toms AP, Marshall TJ, Cahir J, Darrah C, Nolan J, Donell ST, Barker T, Tucker JK (2008) MRI of early symptomatic metal-on-metal total hip arthroplasty: a retrospective review of radiological findings in 20 hips. Clin Radiol 63(1):49
Haddad FS, Thakrar RR, Hart AJ, Skinner JA, Nargol AV, Nolan JF, Gill HS, Murray DW, Blom AW, Case CP (2011) Metal-on-metal bearings: the evidence so far. J Bone Joint Surg Br 93(5):572
Daniel J, Holland J, Quigley L, Sprague S, Bhandari M (2012) Pseudotumors associated with total hip arthroplasty. J Bone Joint Surg Am 94(1):86
Kwon YM, Xia Z, Glyn-Jones S, Beard D, Gill HS, Murray DW (2009) Dose-dependent cytotoxicity of clinically relevant cobalt nanoparticles and ions on macrophages in vitro. Biomed Mater 4(2):025018
Langton DJ, Jameson SS, Joyce TJ, Hallab NJ, Natu S, Nargol AV (2010) Early failure of metal-on-metal bearings in hip resurfacing and large-diameter total hip replacement: a consequence of excess wear. J Bone Joint Surg Br 92(1):38
Cooper HJ, Della Valle CJ, Berger RA, Tetreault M, Paprosky WG, Sporer SM, Jacobs JJ (2012) Corrosion at the head-neck taper as a cause for adverse local tissue reactions after total hip arthroplasty. J Bone Joint Surg Am 94(18):1655
Lindgren JU, Brismar BH, Wikstrom AC (2011) Adverse reaction to metal release from a modular metal-on-polyethylene hip prosthesis. J Bone Joint Surg Br 93(10):1427
Hsu AR, Gross CE, Levine BR (2012) Pseudotumor from modular neck corrosion after ceramic-on-polyethylene total hip arthroplasty. Am J Orthop (Belle Mead NJ) 41(9):422
Stahnke JT, Sharpe KP (2015) Pseudotumor formation in a metal-on-polyethylene total hip arthroplasty due to trunnionosis at the head–neck taper. Surg Technol Int 27:245–250
Hohman DW, Affonso J, Anders M (2011) Ceramic-on-ceramic failure secondary to head–neck taper mismatch. Am J Orthop (Belle Mead NJ) 40(11):571
Pansard E, Fouilleron N, Dereudre G, Migaud H, Girard J (2012) Severe corrosion after malpositioning of a metallic head over the Morse taper of a cementless hip arthroplasty––a case report. Orthop Traumatol Surg Res 98(2):247
Botti TP, Gent J, Martell JM, Manning DW (2005) Trunion fracture of a fully porous-coated femoral stem––case report. J Arthroplasty 20(7):943
The authors or their institution did not receive any financial support for this manuscript.
Conflict of interest
MAM is a consultant for, or has received institutional or research support from the following companies—Sage Products, TissueGene, OnGoing Care Solutions, DJO Global, Microport, Orthosensor, National Institutes of Health, Stryker, Medical Compression Systems, Johnson and Johnson, Pacira Pharmaceuticals, Merz. He is on the editorial/governing board of the American Journal of Orthopedics, Journal of Arthroplasty, Journal of Knee Surgery, and Surgical Technology International.
The other authors have no disclosures to report.
About this article
Cite this article
Mistry, J.B., Chughtai, M., Elmallah, R.K. et al. Trunnionosis in total hip arthroplasty: a review. J Orthopaed Traumatol 17, 1–6 (2016). https://doi.org/10.1007/s10195-016-0391-1
- Total hip arthroplasty